#------------------------------------------------------------------------------
#$Date: 2020-12-09 05:21:26 +0200 (Wed, 09 Dec 2020) $
#$Revision: 259699 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/58/7705895.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7705895
loop_
_publ_author_name
'Jiang, Jia-Ying'
'Xu, Qi'
'Ma, Jia-Jun'
'Gong, Zhi-Xin'
'Shi, Chao'
'Zhang, Yi'
_publ_section_title
;
 Above room-temperature dielectric switching and semiconducting properties
 of a layered organic-inorganic hybrid compound:
 (C₆H₁₂N)₂Pb(NO₃)₄.
;
_journal_issue                   46
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16860
_journal_page_last               16865
_journal_paper_doi               10.1039/d0dt03206a
_journal_volume                  49
_journal_year                    2020
_chemical_formula_moiety         'N4 O12 Pb, 2(C6 H12 N)'
_chemical_formula_sum            'C12 H24 N6 O12 Pb'
_chemical_formula_weight         651.57
_space_group_crystal_system      tetragonal
_space_group_IT_number           139
_space_group_name_Hall           '-I 4 2'
_space_group_name_H-M_alt        'I 4/m m m'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2020-10-22 deposited with the CCDC.	2020-10-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.8961(9)
_cell_length_b                   6.8961(9)
_cell_length_c                   23.195(10)
_cell_measurement_reflns_used    1300
_cell_measurement_temperature    373(2)
_cell_measurement_theta_max      23.7320
_cell_measurement_theta_min      3.0660
_cell_volume                     1103.1(5)
_computing_data_collection       'CrysAlisPro 1.171.40.39a (Rigaku OD, 2019)'
_computing_molecular_graphics    'Diamond 3.2 (Brandenburg, 2014)'
_computing_publication_material  'Word 2018'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      373(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.859
_diffrn_measurement_device_type  Rigaku
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0185
_diffrn_reflns_av_unetI/netI     0.0172
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.859
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -33
_diffrn_reflns_number            2373
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.859
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         31.261
_diffrn_reflns_theta_min         3.082
_exptl_absorpt_coefficient_mu    7.717
_exptl_absorpt_correction_T_max  0.172
_exptl_absorpt_correction_T_min  0.089
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            clourless
_exptl_crystal_density_diffrn    1.962
_exptl_crystal_description       block
_exptl_crystal_F_000             632
_exptl_crystal_size_max          0.397
_exptl_crystal_size_mid          0.246
_exptl_crystal_size_min          0.199
_refine_diff_density_max         0.902
_refine_diff_density_min         -1.580
_refine_diff_density_rms         0.139
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.259
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     84
_refine_ls_number_reflns         504
_refine_ls_number_restraints     100
_refine_ls_restrained_S_all      1.265
_refine_ls_R_factor_all          0.0623
_refine_ls_R_factor_gt           0.0516
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0694P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1092
_refine_ls_wR_factor_ref         0.1132
_reflns_Friedel_coverage         0.000
_reflns_number_gt                417
_reflns_number_total             585
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d0dt03206a2.cif
_cod_data_source_block           HTP
_cod_database_code               7705895
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.166
_shelx_estimated_absorpt_t_max   0.523
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O2 O 0.5000 -0.5000 0.6817(11) 0.219(10) Uani 1 8 d S TU P . .
O3 O 0.5000 -0.655(6) 0.6021(9) 0.31(3) Uani 0.5 2 d S TU P . .
N3 N 0.5000 -0.5000 0.6296(15) 0.184(8) Uani 1 8 d S TU P . .
Pb Pb 0.5000 -0.5000 0.5000 0.0858(4) Uani 1 16 d S TU P . .
C6 C 1.080(8) -0.110(6) 0.6325(16) 0.144(15) Uani 0.125 1 d G U P A -1
C2 C 1.190(8) -0.018(9) 0.6814(17) 0.135(19) Uani 0.125 1 d G U P A -1
H2B H 1.3203 0.0168 0.6695 0.100 Uiso 0.125 1 d G U P A -1
H2A H 1.1973 -0.1050 0.7147 0.100 Uiso 0.125 1 d G U P A -1
C5 C 1.071(9) 0.158(9) 0.6950(19) 0.15(2) Uani 0.125 1 d G U P A -1
H5A H 1.0232 0.1546 0.7347 0.100 Uiso 0.125 1 d G U P A -1
H5B H 1.1445 0.2760 0.6891 0.100 Uiso 0.125 1 d G U P A -1
C9 C 0.910(8) 0.142(8) 0.6529(17) 0.156(18) Uani 0.125 1 d G U P A -1
C10 C 0.893(10) -0.198(8) 0.654(3) 0.17(2) Uani 0.125 1 d G U P A -1
H6 H 1.1582 -0.1969 0.6081 0.100 Uiso 0.125 1 d G U P A -1
N12 N 1.005(8) 0.061(7) 0.6020(12) 0.137(17) Uani 0.125 1 d G U P A -1
C13 C 0.780(8) -0.022(12) 0.667(2) 0.17(2) Uani 0.125 1 d G U P A -1
H9 H 0.8422 0.2644 0.6455 0.100 Uiso 0.125 1 d G U P A -1
H10B H 0.8311 -0.2762 0.6242 0.100 Uiso 0.125 1 d G U P A -1
H10A H 0.9131 -0.2763 0.6885 0.100 Uiso 0.125 1 d G U P A -1
H12A H 1.0989 0.1367 0.5882 0.100 Uiso 0.125 1 d G U P A -1
H12B H 0.9220 0.0302 0.5737 0.100 Uiso 0.125 1 d G U P A -1
H13A H 0.7434 -0.0185 0.7076 0.100 Uiso 0.125 1 d G U P A -1
H13B H 0.6638 -0.0170 0.6433 0.100 Uiso 0.125 1 d G U P A -1
N1_1 N 0.5000 0.0000 0.5000 0.210(13) Uani 1 8 d DS TU P . .
O1_1 O 0.629(4) 0.127(3) 0.5000 0.165(11) Uani 0.25 2 d DS TU P . .
O2_1 O 0.363(5) 0.0000 0.5345(18) 0.26(2) Uani 0.25 2 d DS TU P . .
O3_1 O 0.5000 -0.137(4) 0.4649(13) 0.205(16) Uani 0.25 2 d DS TU P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N3 O3 Pb 96(2) . . ?
O2 N3 O3 120.8(18) . 24_645 ?
O2 N3 O3 120.8(18) . . ?
O3 N3 O3 74.8(16) 24_645 . ?
O2 N3 O3 120.8(18) . 4_655 ?
O3 N3 O3 0(3) 24_645 4_655 ?
O3 N3 O3 74.8(16) . 4_655 ?
O2 N3 O3 120.8(18) . 23 ?
O3 N3 O3 118(4) 24_645 23 ?
O3 N3 O3 74.8(16) . 23 ?
O3 N3 O3 118(4) 4_655 23 ?
O2 N3 O3 120.8(18) . 3_545 ?
O3 N3 O3 118(4) 24_645 3_545 ?
O3 N3 O3 74.8(16) . 3_545 ?
O3 N3 O3 118(4) 4_655 3_545 ?
O3 N3 O3 0.0(16) 23 3_545 ?
O2 N3 O3 120.8(18) . 2_645 ?
O3 N3 O3 74.8(16) 24_645 2_645 ?
O3 N3 O3 118(4) . 2_645 ?
O3 N3 O3 74.8(16) 4_655 2_645 ?
O3 N3 O3 74.8(16) 23 2_645 ?
O3 N3 O3 74.8(16) 3_545 2_645 ?
O3 Pb O3 33.9(12) 19_656 18_556 ?
O3 Pb O3 146.1(12) 19_656 2_645 ?
O3 Pb O3 180.0 18_556 2_645 ?
O3 Pb O3 48.6(18) 19_656 20_546 ?
O3 Pb O3 33.9(12) 18_556 20_546 ?
O3 Pb O3 146.1(13) 2_645 20_546 ?
O3 Pb O3 33.9(12) 19_656 17_646 ?
O3 Pb O3 48.6(18) 18_556 17_646 ?
O3 Pb O3 131.4(18) 2_645 17_646 ?
O3 Pb O3 33.9(12) 20_546 17_646 ?
O3 Pb O3 180.0 19_656 23 ?
O3 Pb O3 146.1(12) 18_556 23 ?
O3 Pb O3 33.9(12) 2_645 23 ?
O3 Pb O3 131.4(18) 20_546 23 ?
O3 Pb O3 146.1(12) 17_646 23 ?
O3 Pb O3 180.0 19_656 3_545 ?
O3 Pb O3 146.1(12) 18_556 3_545 ?
O3 Pb O3 33.9(12) 2_645 3_545 ?
O3 Pb O3 131.4(18) 20_546 3_545 ?
O3 Pb O3 146.1(12) 17_646 3_545 ?
O3 Pb O3 0.0(18) 23 3_545 ?
O3 Pb O3 131.4(18) 19_656 4_655 ?
O3 Pb O3 146.1(12) 18_556 4_655 ?
O3 Pb O3 33.9(12) 2_645 4_655 ?
O3 Pb O3 180.0 20_546 4_655 ?
O3 Pb O3 146.1(12) 17_646 4_655 ?
O3 Pb O3 48.6(18) 23 4_655 ?
O3 Pb O3 48.6(18) 3_545 4_655 ?
O3 Pb O3 131.4(18) 19_656 24_645 ?
O3 Pb O3 146.1(12) 18_556 24_645 ?
O3 Pb O3 33.9(12) 2_645 24_645 ?
O3 Pb O3 180.0 20_546 24_645 ?
O3 Pb O3 146.1(12) 17_646 24_645 ?
O3 Pb O3 48.6(18) 23 24_645 ?
O3 Pb O3 48.6(18) 3_545 24_645 ?
O3 Pb O3 0.0(17) 4_655 24_645 ?
O3 Pb O3 146.1(12) 19_656 . ?
O3 Pb O3 131.4(18) 18_556 . ?
O3 Pb O3 48.6(18) 2_645 . ?
O3 Pb O3 146.1(12) 20_546 . ?
O3 Pb O3 180.0 17_646 . ?
O3 Pb O3 33.9(12) 23 . ?
O3 Pb O3 33.9(12) 3_545 . ?
O3 Pb O3 33.9(12) 4_655 . ?
O3 Pb O3 33.9(12) 24_645 . ?
O3 Pb O3_1 106.4(5) 19_656 5_656 ?
O3 Pb O3_1 132.3(10) 18_556 5_656 ?
O3 Pb O3_1 47.7(10) 2_645 5_656 ?
O3 Pb O3_1 106.4(5) 20_546 5_656 ?
O3 Pb O3_1 83.7(11) 17_646 5_656 ?
O3 Pb O3_1 73.6(5) 23 5_656 ?
O3 Pb O3_1 73.6(5) 3_545 5_656 ?
O3 Pb O3_1 73.6(5) 4_655 5_656 ?
O3 Pb O3_1 73.6(5) 24_645 5_656 ?
O3 Pb O3_1 96.3(11) . 5_656 ?
O3 Pb O3_1 73.6(5) 19_656 . ?
O3 Pb O3_1 96.3(11) 18_556 . ?
O3 Pb O3_1 83.7(11) 2_645 . ?
O3 Pb O3_1 73.6(5) 20_546 . ?
O3 Pb O3_1 47.7(10) 17_646 . ?
O3 Pb O3_1 106.4(5) 23 . ?
O3 Pb O3_1 106.4(5) 3_545 . ?
O3 Pb O3_1 106.4(5) 4_655 . ?
O3 Pb O3_1 106.4(5) 24_645 . ?
O3 Pb O3_1 132.3(10) . . ?
O3_1 Pb O3_1 36.0(10) 5_656 . ?
N12 C6 C2 101.8 . . ?
N12 C6 C10 100.3 . . ?
C2 C6 C10 110.4 . . ?
C5 C2 C6 102.9 . . ?
C9 C5 C2 102.2 . . ?
N12 C9 C13 98.92(6) . . ?
N12 C9 C5 103.0 . . ?
C13 C9 C5 111.2 . . ?
C13 C10 C6 100.72(6) . . ?
C9 N12 C6 94.5 . . ?
C10 C13 C9 105.6 . . ?
O2_1 N1_1 O2_1 80(5) 6_556 . ?
O2_1 N1_1 O2_1 179.999(15) 6_556 2_655 ?
O2_1 N1_1 O2_1 100(5) . 2_655 ?
O2_1 N1_1 O2_1 100(5) 6_556 17_656 ?
O2_1 N1_1 O2_1 179.999(14) . 17_656 ?
O2_1 N1_1 O2_1 80(5) 2_655 17_656 ?
O2_1 N1_1 O1_1 57.0(17) 6_556 17_656 ?
O2_1 N1_1 O1_1 57.0(17) . 17_656 ?
O2_1 N1_1 O1_1 123.0(17) 2_655 17_656 ?
O2_1 N1_1 O1_1 123.0(17) 17_656 17_656 ?
O2_1 N1_1 O1_1 123.0(17) 6_556 21 ?
O2_1 N1_1 O1_1 123.0(17) . 21 ?
O2_1 N1_1 O1_1 57.0(16) 2_655 21 ?
O2_1 N1_1 O1_1 57.0(16) 17_656 21 ?
O1_1 N1_1 O1_1 91(3) 17_656 21 ?
O2_1 N1_1 O1_1 57.0(16) 6_556 5_656 ?
O2_1 N1_1 O1_1 57.0(16) . 5_656 ?
O2_1 N1_1 O1_1 123.0(16) 2_655 5_656 ?
O2_1 N1_1 O1_1 123.0(17) 17_656 5_656 ?
O1_1 N1_1 O1_1 89(3) 17_656 5_656 ?
O1_1 N1_1 O1_1 180.000(17) 21 5_656 ?
O2_1 N1_1 O1_1 123.0(17) 6_556 . ?
O2_1 N1_1 O1_1 123.0(17) . . ?
O2_1 N1_1 O1_1 57.0(17) 2_655 . ?
O2_1 N1_1 O1_1 57.0(17) 17_656 . ?
O1_1 N1_1 O1_1 180.0 17_656 . ?
O1_1 N1_1 O1_1 89(3) 21 . ?
O1_1 N1_1 O1_1 91(3) 5_656 . ?
O2_1 N1_1 O3_1 65.1(16) 6_556 . ?
O2_1 N1_1 O3_1 114.9(16) . . ?
O2_1 N1_1 O3_1 114.9(16) 2_655 . ?
O2_1 N1_1 O3_1 65.1(16) 17_656 . ?
O1_1 N1_1 O3_1 57.9(12) 17_656 . ?
O1_1 N1_1 O3_1 57.9(12) 21 . ?
O1_1 N1_1 O3_1 122.1(12) 5_656 . ?
O1_1 N1_1 O3_1 122.1(12) . . ?
O2_1 N1_1 O3_1 114.9(16) 6_556 5_656 ?
O2_1 N1_1 O3_1 65.1(16) . 5_656 ?
O2_1 N1_1 O3_1 65.1(16) 2_655 5_656 ?
O2_1 N1_1 O3_1 114.9(16) 17_656 5_656 ?
O1_1 N1_1 O3_1 57.9(12) 17_656 5_656 ?
O1_1 N1_1 O3_1 57.9(12) 21 5_656 ?
O1_1 N1_1 O3_1 122.1(12) 5_656 5_656 ?
O1_1 N1_1 O3_1 122.1(12) . 5_656 ?
O3_1 N1_1 O3_1 82(4) . 5_656 ?
O2_1 N1_1 O3_1 114.9(16) 6_556 17_656 ?
O2_1 N1_1 O3_1 65.1(16) . 17_656 ?
O2_1 N1_1 O3_1 65.1(16) 2_655 17_656 ?
O2_1 N1_1 O3_1 114.9(16) 17_656 17_656 ?
O1_1 N1_1 O3_1 122.1(12) 17_656 17_656 ?
O1_1 N1_1 O3_1 122.1(12) 21 17_656 ?
O1_1 N1_1 O3_1 57.9(12) 5_656 17_656 ?
O1_1 N1_1 O3_1 57.9(12) . 17_656 ?
O3_1 N1_1 O3_1 179.997(11) . 17_656 ?
O3_1 N1_1 O3_1 98(4) 5_656 17_656 ?
O2_1 N1_1 O3_1 65.1(16) 6_556 2_655 ?
O2_1 N1_1 O3_1 114.9(16) . 2_655 ?
O2_1 N1_1 O3_1 114.9(16) 2_655 2_655 ?
O2_1 N1_1 O3_1 65.1(16) 17_656 2_655 ?
O1_1 N1_1 O3_1 122.1(12) 17_656 2_655 ?
O1_1 N1_1 O3_1 122.1(12) 21 2_655 ?
O1_1 N1_1 O3_1 57.9(12) 5_656 2_655 ?
O1_1 N1_1 O3_1 57.9(12) . 2_655 ?
O3_1 N1_1 O3_1 98(4) . 2_655 ?
O3_1 N1_1 O3_1 180.0 5_656 2_655 ?
O3_1 N1_1 O3_1 82(4) 17_656 2_655 ?
O2_1 O1_1 O2_1 85(3) 17_656 2_655 ?
O2_1 O1_1 O3_1 68(3) 17_656 2_655 ?
O2_1 O1_1 O3_1 122.4(16) 2_655 2_655 ?
O2_1 O1_1 O3_1 122.4(16) 17_656 17_656 ?
O2_1 O1_1 O3_1 68(3) 2_655 17_656 ?
O3_1 O1_1 O3_1 85(3) 2_655 17_656 ?
O2_1 O1_1 N1_1 61.3(11) 17_656 . ?
O2_1 O1_1 N1_1 61.3(11) 2_655 . ?
O3_1 O1_1 N1_1 61.1(10) 2_655 . ?
O3_1 O1_1 N1_1 61.1(10) 17_656 . ?
O2_1 O1_1 O1_1 42.6(15) 17_656 21 ?
O2_1 O1_1 O1_1 42.6(15) 2_655 21 ?
O3_1 O1_1 O1_1 93.4(18) 2_655 21 ?
O3_1 O1_1 O1_1 93.4(18) 17_656 21 ?
N1_1 O1_1 O1_1 45.4(14) . 21 ?
O2_1 O1_1 O1_1 93(2) 17_656 5_656 ?
O2_1 O1_1 O1_1 93(2) 2_655 5_656 ?
O3_1 O1_1 O1_1 42.7(12) 2_655 5_656 ?
O3_1 O1_1 O1_1 42.7(12) 17_656 5_656 ?
N1_1 O1_1 O1_1 44.6(14) . 5_656 ?
O1_1 O1_1 O1_1 89.999(8) 21 5_656 ?
O2_1 O1_1 Pb 135(2) 17_656 1_565 ?
O2_1 O1_1 Pb 135(2) 2_655 1_565 ?
O3_1 O1_1 Pb 73(2) 2_655 1_565 ?
O3_1 O1_1 Pb 73(2) 17_656 1_565 ?
N1_1 O1_1 Pb 115.6(17) . 1_565 ?
O1_1 O1_1 Pb 161.0(4) 21 1_565 ?
O1_1 O1_1 Pb 71.0(4) 5_656 1_565 ?
O1_1 O2_1 O1_1 95(3) 17_656 5_656 ?
O1_1 O2_1 N1_1 61.6(11) 17_656 . ?
O1_1 O2_1 N1_1 61.6(11) 5_656 . ?
O1_1 O2_1 O3_1 56.7(19) 17_656 5_656 ?
O1_1 O2_1 O3_1 119.3(14) 5_656 5_656 ?
N1_1 O2_1 O3_1 57.7(10) . 5_656 ?
O1_1 O2_1 O3_1 119.3(14) 17_656 17_656 ?
O1_1 O2_1 O3_1 56.7(19) 5_656 17_656 ?
N1_1 O2_1 O3_1 57.7(10) . 17_656 ?
O3_1 O2_1 O3_1 90(3) 5_656 17_656 ?
O1_1 O2_1 O2_1 47.5(17) 17_656 6_556 ?
O1_1 O2_1 O2_1 47.5(17) 5_656 6_556 ?
N1_1 O2_1 O2_1 50(3) . 6_556 ?
O3_1 O2_1 O2_1 91(2) 5_656 6_556 ?
O3_1 O2_1 O2_1 91(2) 17_656 6_556 ?
O1_1 O3_1 O1_1 95(2) 21 17_656 ?
O1_1 O3_1 N1_1 61.0(9) 21 . ?
O1_1 O3_1 N1_1 61.0(9) 17_656 . ?
O1_1 O3_1 O2_1 118.2(15) 21 6_556 ?
O1_1 O3_1 O2_1 55(2) 17_656 6_556 ?
N1_1 O3_1 O2_1 57.3(10) . 6_556 ?
O1_1 O3_1 O2_1 55(2) 21 17_656 ?
O1_1 O3_1 O2_1 118.2(15) 17_656 17_656 ?
N1_1 O3_1 O2_1 57.3(10) . 17_656 ?
O2_1 O3_1 O2_1 90(3) 6_556 17_656 ?
O1_1 O3_1 O3_1 47.5(14) 21 5_656 ?
O1_1 O3_1 O3_1 47.5(14) 17_656 5_656 ?
N1_1 O3_1 O3_1 49.2(18) . 5_656 ?
O2_1 O3_1 O3_1 89(2) 6_556 5_656 ?
O2_1 O3_1 O3_1 89(2) 17_656 5_656 ?
O1_1 O3_1 Pb 81(2) 21 . ?
O1_1 O3_1 Pb 81(2) 17_656 . ?
N1_1 O3_1 Pb 121(2) . . ?
O2_1 O3_1 Pb 132(2) 6_556 . ?
O2_1 O3_1 Pb 132(2) 17_656 . ?
O3_1 O3_1 Pb 72.0(5) 5_656 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O2 N3 1.21(4) . ?
O3 N3 1.25(4) . ?
O3 Pb 2.60(2) . ?
N3 O3 1.25(4) 24_645 ?
N3 O3 1.25(4) 4_655 ?
N3 O3 1.25(4) 23 ?
N3 O3 1.25(4) 3_545 ?
N3 O3 1.25(4) 2_645 ?
Pb O3 2.60(2) 19_656 ?
Pb O3 2.60(2) 18_556 ?
Pb O3 2.60(2) 2_645 ?
Pb O3 2.60(2) 20_546 ?
Pb O3 2.60(2) 17_646 ?
Pb O3 2.60(2) 23 ?
Pb O3 2.60(2) 3_545 ?
Pb O3 2.60(2) 4_655 ?
Pb O3 2.60(2) 24_645 ?
Pb O3_1 2.63(3) 5_656 ?
Pb O3_1 2.63(3) . ?
C6 N12 1.4664 . ?
C6 C2 1.5030 . ?
C6 C10 1.5121 . ?
C2 C5 1.4995 . ?
C5 C9 1.4830 . ?
C9 N12 1.4621 . ?
C9 C13 1.4766 . ?
C10 C13 1.4708 . ?
N1_1 O2_1 1.240(15) 6_556 ?
N1_1 O2_1 1.240(15) . ?
N1_1 O2_1 1.240(15) 2_655 ?
N1_1 O2_1 1.240(15) 17_656 ?
N1_1 O1_1 1.244(15) 17_656 ?
N1_1 O1_1 1.244(15) 21 ?
N1_1 O1_1 1.244(15) 5_656 ?
N1_1 O1_1 1.244(15) . ?
N1_1 O3_1 1.246(15) . ?
N1_1 O3_1 1.246(15) 5_656 ?
N1_1 O3_1 1.246(15) 17_656 ?
N1_1 O3_1 1.246(15) 2_655 ?
O1_1 O2_1 1.19(3) 17_656 ?
O1_1 O2_1 1.19(3) 2_655 ?
O1_1 O3_1 1.21(3) 2_655 ?
O1_1 O3_1 1.21(3) 17_656 ?
O1_1 O1_1 1.75(5) 21 ?
O1_1 O1_1 1.77(5) 5_656 ?
O1_1 Pb 2.72(3) 1_565 ?
O2_1 O1_1 1.19(3) 17_656 ?
O2_1 O1_1 1.19(3) 5_656 ?
O2_1 O3_1 1.34(3) 5_656 ?
O2_1 O3_1 1.34(3) 17_656 ?
O2_1 O2_1 1.60(8) 6_556 ?
O3_1 O1_1 1.21(3) 21 ?
O3_1 O1_1 1.21(3) 17_656 ?
O3_1 O2_1 1.34(3) 6_556 ?
O3_1 O2_1 1.34(3) 17_656 ?
O3_1 O3_1 1.63(6) 5_656 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Pb O3 N3 O2 180.000(5) . . . . ?
Pb O3 N3 O3 62.9(12) . . . 24_645 ?
Pb O3 N3 O3 62.9(12) . . . 4_655 ?
Pb O3 N3 O3 -62.9(12) . . . 23 ?
Pb O3 N3 O3 -62.9(12) . . . 3_545 ?
Pb O3 N3 O3 0.000(10) . . . 2_645 ?
N12 C6 C2 C5 34.4 . . . . ?
C10 C6 C2 C5 -71.5 . . . . ?
C6 C2 C5 C9 0.5 . . . . ?
C2 C5 C9 N12 -35.6 . . . . ?
C2 C5 C9 C13 69.5 . . . . ?
N12 C6 C10 C13 -35.9 . . . . ?
C2 C6 C10 C13 71.0 . . . . ?
C13 C9 N12 C6 -58.2 . . . . ?
C5 C9 N12 C6 56.12(5) . . . . ?
C2 C6 N12 C9 -54.92(5) . . . . ?
C10 C6 N12 C9 58.7 . . . . ?
C6 C10 C13 C9 -0.7 . . . . ?
N12 C9 C13 C10 37.1 . . . . ?
C5 C9 C13 C10 -70.7 . . . . ?
O2_1 N1_1 O1_1 O2_1 -79(5) 6_556 . . 17_656 ?
O2_1 N1_1 O1_1 O2_1 179.999(1) . . . 17_656 ?
O2_1 N1_1 O1_1 O2_1 101(5) 2_655 . . 17_656 ?
O1_1 N1_1 O1_1 O2_1 50(3) 21 . . 17_656 ?
O1_1 N1_1 O1_1 O2_1 -130(3) 5_656 . . 17_656 ?
O3_1 N1_1 O1_1 O2_1 0(4) . . . 17_656 ?
O3_1 N1_1 O1_1 O2_1 101(3) 5_656 . . 17_656 ?
O3_1 N1_1 O1_1 O2_1 180(4) 17_656 . . 17_656 ?
O3_1 N1_1 O1_1 O2_1 -79(3) 2_655 . . 17_656 ?
O2_1 N1_1 O1_1 O2_1 180.001(0) 6_556 . . 2_655 ?
O2_1 N1_1 O1_1 O2_1 79(5) . . . 2_655 ?
O2_1 N1_1 O1_1 O2_1 -101(5) 17_656 . . 2_655 ?
O1_1 N1_1 O1_1 O2_1 -50(3) 21 . . 2_655 ?
O1_1 N1_1 O1_1 O2_1 130(3) 5_656 . . 2_655 ?
O3_1 N1_1 O1_1 O2_1 -101(3) . . . 2_655 ?
O3_1 N1_1 O1_1 O2_1 0(4) 5_656 . . 2_655 ?
O3_1 N1_1 O1_1 O2_1 79(3) 17_656 . . 2_655 ?
O3_1 N1_1 O1_1 O2_1 -180(4) 2_655 . . 2_655 ?
O2_1 N1_1 O1_1 O3_1 0(4) 6_556 . . 2_655 ?
O2_1 N1_1 O1_1 O3_1 -101(3) . . . 2_655 ?
O2_1 N1_1 O1_1 O3_1 180(4) 2_655 . . 2_655 ?
O2_1 N1_1 O1_1 O3_1 79(3) 17_656 . . 2_655 ?
O1_1 N1_1 O1_1 O3_1 130(2) 21 . . 2_655 ?
O1_1 N1_1 O1_1 O3_1 -50(2) 5_656 . . 2_655 ?
O3_1 N1_1 O1_1 O3_1 79(4) . . . 2_655 ?
O3_1 N1_1 O1_1 O3_1 179.997(1) 5_656 . . 2_655 ?
O3_1 N1_1 O1_1 O3_1 -101(4) 17_656 . . 2_655 ?
O2_1 N1_1 O1_1 O3_1 101(3) 6_556 . . 17_656 ?
O2_1 N1_1 O1_1 O3_1 0(4) . . . 17_656 ?
O2_1 N1_1 O1_1 O3_1 -79(3) 2_655 . . 17_656 ?
O2_1 N1_1 O1_1 O3_1 -180(4) 17_656 . . 17_656 ?
O1_1 N1_1 O1_1 O3_1 -130(2) 21 . . 17_656 ?
O1_1 N1_1 O1_1 O3_1 50(2) 5_656 . . 17_656 ?
O3_1 N1_1 O1_1 O3_1 180.003(0) . . . 17_656 ?
O3_1 N1_1 O1_1 O3_1 -79(4) 5_656 . . 17_656 ?
O3_1 N1_1 O1_1 O3_1 101(4) 2_655 . . 17_656 ?
O2_1 N1_1 O1_1 O1_1 -130(3) 6_556 . . 21 ?
O2_1 N1_1 O1_1 O1_1 130(3) . . . 21 ?
O2_1 N1_1 O1_1 O1_1 50(3) 2_655 . . 21 ?
O2_1 N1_1 O1_1 O1_1 -50(3) 17_656 . . 21 ?
O1_1 N1_1 O1_1 O1_1 180.0 5_656 . . 21 ?
O3_1 N1_1 O1_1 O1_1 -50(2) . . . 21 ?
O3_1 N1_1 O1_1 O1_1 50(2) 5_656 . . 21 ?
O3_1 N1_1 O1_1 O1_1 130(2) 17_656 . . 21 ?
O3_1 N1_1 O1_1 O1_1 -130(2) 2_655 . . 21 ?
O2_1 N1_1 O1_1 O1_1 50(3) 6_556 . . 5_656 ?
O2_1 N1_1 O1_1 O1_1 -50(3) . . . 5_656 ?
O2_1 N1_1 O1_1 O1_1 -130(3) 2_655 . . 5_656 ?
O2_1 N1_1 O1_1 O1_1 130(3) 17_656 . . 5_656 ?
O1_1 N1_1 O1_1 O1_1 180.0 21 . . 5_656 ?
O3_1 N1_1 O1_1 O1_1 130(2) . . . 5_656 ?
O3_1 N1_1 O1_1 O1_1 -130(2) 5_656 . . 5_656 ?
O3_1 N1_1 O1_1 O1_1 -50(2) 17_656 . . 5_656 ?
O3_1 N1_1 O1_1 O1_1 50(2) 2_655 . . 5_656 ?
O2_1 N1_1 O1_1 Pb 50(3) 6_556 . . 1_565 ?
O2_1 N1_1 O1_1 Pb -50(3) . . . 1_565 ?
O2_1 N1_1 O1_1 Pb -130(3) 2_655 . . 1_565 ?
O2_1 N1_1 O1_1 Pb 130(3) 17_656 . . 1_565 ?
O1_1 N1_1 O1_1 Pb 180.0 21 . . 1_565 ?
O1_1 N1_1 O1_1 Pb 0.0 5_656 . . 1_565 ?
O3_1 N1_1 O1_1 Pb 130(2) . . . 1_565 ?
O3_1 N1_1 O1_1 Pb -130(2) 5_656 . . 1_565 ?
O3_1 N1_1 O1_1 Pb -50(2) 17_656 . . 1_565 ?
O3_1 N1_1 O1_1 Pb 50(2) 2_655 . . 1_565 ?
O2_1 N1_1 O2_1 O1_1 56.7(19) 6_556 . . 17_656 ?
O2_1 N1_1 O2_1 O1_1 -123.3(19) 2_655 . . 17_656 ?
O1_1 N1_1 O2_1 O1_1 -67(4) 21 . . 17_656 ?
O1_1 N1_1 O2_1 O1_1 113(4) 5_656 . . 17_656 ?
O1_1 N1_1 O2_1 O1_1 179.999(1) . . . 17_656 ?
O3_1 N1_1 O2_1 O1_1 0(3) . . . 17_656 ?
O3_1 N1_1 O2_1 O1_1 -67(2) 5_656 . . 17_656 ?
O3_1 N1_1 O2_1 O1_1 -180(3) 17_656 . . 17_656 ?
O3_1 N1_1 O2_1 O1_1 113(2) 2_655 . . 17_656 ?
O2_1 N1_1 O2_1 O1_1 -56.7(19) 6_556 . . 5_656 ?
O2_1 N1_1 O2_1 O1_1 123.3(19) 2_655 . . 5_656 ?
O1_1 N1_1 O2_1 O1_1 -113(4) 17_656 . . 5_656 ?
O1_1 N1_1 O2_1 O1_1 180.00(2) 21 . . 5_656 ?
O1_1 N1_1 O2_1 O1_1 67(4) . . . 5_656 ?
O3_1 N1_1 O2_1 O1_1 -113(2) . . . 5_656 ?
O3_1 N1_1 O2_1 O1_1 180(3) 5_656 . . 5_656 ?
O3_1 N1_1 O2_1 O1_1 67(2) 17_656 . . 5_656 ?
O3_1 N1_1 O2_1 O1_1 0(3) 2_655 . . 5_656 ?
O2_1 N1_1 O2_1 O3_1 123(2) 6_556 . . 5_656 ?
O2_1 N1_1 O2_1 O3_1 -57(2) 2_655 . . 5_656 ?
O1_1 N1_1 O2_1 O3_1 67(2) 17_656 . . 5_656 ?
O1_1 N1_1 O2_1 O3_1 0(3) 21 . . 5_656 ?
O1_1 N1_1 O2_1 O3_1 -180(3) 5_656 . . 5_656 ?
O1_1 N1_1 O2_1 O3_1 -113(2) . . . 5_656 ?
O3_1 N1_1 O2_1 O3_1 67(4) . . . 5_656 ?
O3_1 N1_1 O2_1 O3_1 -113(4) 17_656 . . 5_656 ?
O3_1 N1_1 O2_1 O3_1 179.997(17) 2_655 . . 5_656 ?
O2_1 N1_1 O2_1 O3_1 -123(2) 6_556 . . 17_656 ?
O2_1 N1_1 O2_1 O3_1 57(2) 2_655 . . 17_656 ?
O1_1 N1_1 O2_1 O3_1 180(3) 17_656 . . 17_656 ?
O1_1 N1_1 O2_1 O3_1 113(2) 21 . . 17_656 ?
O1_1 N1_1 O2_1 O3_1 -67(2) 5_656 . . 17_656 ?
O1_1 N1_1 O2_1 O3_1 0(3) . . . 17_656 ?
O3_1 N1_1 O2_1 O3_1 179.997(1) . . . 17_656 ?
O3_1 N1_1 O2_1 O3_1 113(4) 5_656 . . 17_656 ?
O3_1 N1_1 O2_1 O3_1 -67(4) 2_655 . . 17_656 ?
O2_1 N1_1 O2_1 O2_1 180.000(18) 2_655 . . 6_556 ?
O1_1 N1_1 O2_1 O2_1 -56.7(19) 17_656 . . 6_556 ?
O1_1 N1_1 O2_1 O2_1 -123.3(19) 21 . . 6_556 ?
O1_1 N1_1 O2_1 O2_1 56.7(19) 5_656 . . 6_556 ?
O1_1 N1_1 O2_1 O2_1 123.3(19) . . . 6_556 ?
O3_1 N1_1 O2_1 O2_1 -57(2) . . . 6_556 ?
O3_1 N1_1 O2_1 O2_1 -123(2) 5_656 . . 6_556 ?
O3_1 N1_1 O2_1 O2_1 123(2) 17_656 . . 6_556 ?
O3_1 N1_1 O2_1 O2_1 57(2) 2_655 . . 6_556 ?
O2_1 N1_1 O3_1 O1_1 -180(3) 6_556 . . 21 ?
O2_1 N1_1 O3_1 O1_1 -115(3) . . . 21 ?
O2_1 N1_1 O3_1 O1_1 0(3) 2_655 . . 21 ?
O2_1 N1_1 O3_1 O1_1 65(3) 17_656 . . 21 ?
O1_1 N1_1 O3_1 O1_1 -115(3) 17_656 . . 21 ?
O1_1 N1_1 O3_1 O1_1 180.000(18) 5_656 . . 21 ?
O1_1 N1_1 O3_1 O1_1 65(3) . . . 21 ?
O3_1 N1_1 O3_1 O1_1 -57.3(17) 5_656 . . 21 ?
O3_1 N1_1 O3_1 O1_1 122.7(17) 2_655 . . 21 ?
O2_1 N1_1 O3_1 O1_1 -65(3) 6_556 . . 17_656 ?
O2_1 N1_1 O3_1 O1_1 0(3) . . . 17_656 ?
O2_1 N1_1 O3_1 O1_1 115(3) 2_655 . . 17_656 ?
O2_1 N1_1 O3_1 O1_1 180(3) 17_656 . . 17_656 ?
O1_1 N1_1 O3_1 O1_1 115(3) 21 . . 17_656 ?
O1_1 N1_1 O3_1 O1_1 -65(3) 5_656 . . 17_656 ?
O1_1 N1_1 O3_1 O1_1 180.001(1) . . . 17_656 ?
O3_1 N1_1 O3_1 O1_1 57.3(17) 5_656 . . 17_656 ?
O3_1 N1_1 O3_1 O1_1 -122.7(17) 2_655 . . 17_656 ?
O2_1 N1_1 O3_1 O2_1 65(5) . . . 6_556 ?
O2_1 N1_1 O3_1 O2_1 180.001(12) 2_655 . . 6_556 ?
O2_1 N1_1 O3_1 O2_1 -115(5) 17_656 . . 6_556 ?
O1_1 N1_1 O3_1 O2_1 65(3) 17_656 . . 6_556 ?
O1_1 N1_1 O3_1 O2_1 180(3) 21 . . 6_556 ?
O1_1 N1_1 O3_1 O2_1 0(3) 5_656 . . 6_556 ?
O1_1 N1_1 O3_1 O2_1 -115(3) . . . 6_556 ?
O3_1 N1_1 O3_1 O2_1 123(2) 5_656 . . 6_556 ?
O3_1 N1_1 O3_1 O2_1 -57(2) 2_655 . . 6_556 ?
O2_1 N1_1 O3_1 O2_1 115(5) 6_556 . . 17_656 ?
O2_1 N1_1 O3_1 O2_1 180.001(0) . . . 17_656 ?
O2_1 N1_1 O3_1 O2_1 -65(5) 2_655 . . 17_656 ?
O1_1 N1_1 O3_1 O2_1 -180(3) 17_656 . . 17_656 ?
O1_1 N1_1 O3_1 O2_1 -65(3) 21 . . 17_656 ?
O1_1 N1_1 O3_1 O2_1 115(3) 5_656 . . 17_656 ?
O1_1 N1_1 O3_1 O2_1 0(3) . . . 17_656 ?
O3_1 N1_1 O3_1 O2_1 -123(2) 5_656 . . 17_656 ?
O3_1 N1_1 O3_1 O2_1 57(2) 2_655 . . 17_656 ?
O2_1 N1_1 O3_1 O3_1 -123(2) 6_556 . . 5_656 ?
O2_1 N1_1 O3_1 O3_1 -57(2) . . . 5_656 ?
O2_1 N1_1 O3_1 O3_1 57(2) 2_655 . . 5_656 ?
O2_1 N1_1 O3_1 O3_1 123(2) 17_656 . . 5_656 ?
O1_1 N1_1 O3_1 O3_1 -57.3(17) 17_656 . . 5_656 ?
O1_1 N1_1 O3_1 O3_1 57.3(17) 21 . . 5_656 ?
O1_1 N1_1 O3_1 O3_1 -122.7(17) 5_656 . . 5_656 ?
O1_1 N1_1 O3_1 O3_1 122.7(17) . . . 5_656 ?
O3_1 N1_1 O3_1 O3_1 180.000(14) 2_655 . . 5_656 ?
O2_1 N1_1 O3_1 Pb -123(2) 6_556 . . . ?
O2_1 N1_1 O3_1 Pb -57(2) . . . . ?
O2_1 N1_1 O3_1 Pb 57(2) 2_655 . . . ?
O2_1 N1_1 O3_1 Pb 123(2) 17_656 . . . ?
O1_1 N1_1 O3_1 Pb -57.3(17) 17_656 . . . ?
O1_1 N1_1 O3_1 Pb 57.3(17) 21 . . . ?
O1_1 N1_1 O3_1 Pb -122.7(17) 5_656 . . . ?
O1_1 N1_1 O3_1 Pb 122.7(17) . . . . ?
O3_1 N1_1 O3_1 Pb 0.000(3) 5_656 . . . ?
O3_1 N1_1 O3_1 Pb 180.000(3) 2_655 . . . ?
